Home >Documents >CEMENT CONCRETE MIX DESIGN - Dronacharyagn.dronacharya.info/.../Unit-1/cc-mix-design-by-klp.pdf ·...

Date post: | 13-Mar-2018 |

Category: | ## Documents |

View: | 252 times |

Download: | 9 times |

Share this document with a friend

Transcript:

CEMENT CONCRETE MIX DESIGNCEMENT CONCRETE MIX DESIGN

DEFINITION

The process of selecting suitable ingredients of concrete

and determining their relative quantities with the

objective of producing a concrete of the required

strength, durability, and workability as economically as

possible, is termed the concrete mix design

1. Nominal Mixes In the past the specifications for concrete prescribed the proportions of cement, fine and coarse aggregates. These mixes of fixed cement-aggregate ratio which ensures adequate strength are termed nominal mixes. These offer simplicity and under normal circumstances, have a margin of strength above that specified. However, due to the variability of mix ingredients the nominal concrete for a given workability varies widely in strength

Types of Mixes

Nominal mix concrete

Traditional way of mix proportion specified in terms of fixed

ratios of Cement : Sand : coarse aggregate (In general by

volume)

4

C5

02

.5

Useful for small works

Useful for routine concrete construction

Limited up to M20 grade

Requires high cement content

The nominal mixes of fixed cement-aggregate ratio (by volume) vary widely in strength and may result in under- or over-rich mixes. For this reason, the minimum compressive strength has been included in many specifications. These mixes are termed standard mixes.

Standard mixes

IS 456-2000 has designated the concrete mixes into a

number of grades as M10, M15, M20, M25, M30, M35

and M40. In this designation the letter M refers to the mix

and the number to the specified 28 day cube strength of

mix in N/mm2. The mixes of grades M10, M15, M20 and

M25 correspond approximately to the mix proportions

(1:3:6), (1:2:4), (1:1.5:3) and (1:1:2) respectively.

The proportions generally adopted are as given below

7

C5

02

.5

Grade of

Concrete

Nominal Mix

proportions

(Cement: FA : CA)

M 5 1:5:10

M7.5 1:4:8

M10 1:3:6

M15 1:2:4

M20 1:1.5:3

DESIGNED MIXES

In these mixes the performance of the concrete is

specified by the designer but the mix proportions are

determined by the producer of concrete, except that the

minimum cement content can be laid down. This is most

rational approach to the selection of mix proportions with

specific materials in mind possessing more or less

unique characteristics.

Several methods of mix design evolved over the

years in different countries

Ex: ACI practice, British practice, Indian

Standard recommendations. etc.

DESIGN MIX CONCRETE

RECOMMENDATIONS FOR CONCRETE MIX

DESIGN ARE GIVEN IN

I.S.10262-1982 & I.S.10262-2009

S.P.-23-1982

Designed mix should meet the design

requirements in the fresh and hardened states

FACTORS AFFECTING THE CHOICE OF MIX

PROPORTIONS The various factors affecting the mix design are:

1. Compressive strength

It is one of the most important properties of concrete and

influences many other describable properties of the

hardened concrete. The mean compressive strength

required at a specific age, usually 28 days, determines

the nominal water-cement ratio of the mix. The other

factor affecting the strength of concrete at a given age

and cured at a prescribed temperature is the degree of

compaction. According to Abrahams law the strength of

fully compacted concrete is inversely proportional to the

water-cement ratio.

2. Workability

The degree of workability required depends on

three factors. These are the size of the section to

be concreted, the amount of reinforcement, and the

method of compaction to be used. For the narrow

and complicated section with numerous corners or

inaccessible parts, the concrete must have a high

workability so that full compaction can be achieved

with a reasonable amount of effort. This also

applies to the embedded steel sections. The

desired workability depends on the compacting

equipment available at the site.

3. Durability

The durability of concrete is its resistance to the

aggressive environmental conditions. High strength

concrete is generally more durable than low

strength concrete. In the situations when the high

strength is not necessary but the conditions of

exposure are such that high durability is vital, the

durability requirement will determine the water-

cement ratio to be used.

4. Maximum nominal size of aggregate

In general, larger the maximum size of aggregate,

smaller is the cement requirement for a particular

water-cement ratio, because the workability of

concrete increases with increase in maximum size

of the aggregate. However, the compressive

strength tends to increase with the decrease in size

of aggregate.

IS 456:2000 and IS 1343:1980 recommend that the

nominal size of the aggregate should be as large as

possible.

5. GRADING AND TYPE OF AGGREGATE

The grading of aggregate influences the mix proportions

for a specified workability and water-cement ratio. Coarser the grading leaner will be mix which can be used. Very lean mix is not desirable since it does not contain enough finer material to make the concrete cohesive.

The type of aggregate influences strongly the aggregate-cement ratio for the desired workability and stipulated water cement ratio. An important feature of a satisfactory aggregate is the uniformity of the grading which can be achieved by mixing different size fractions.

6. QUALITY CONTROL

The degree of control can be estimated statistically

by the variations in test results. The variation in

strength results from the variations in the properties

of the mix ingredients and lack of control of

accuracy in batching, mixing, placing, curing and

testing. The lower the difference between the mean

and minimum strengths of the mix lower will be the

cement-content required. The factor controlling this

difference is termed as quality control.

MIX PROPORTION DESIGNATIONS

The common method of expressing the proportions

of ingredients of a concrete mix is in the terms of

parts or ratios of cement, fine and coarse

aggregates. For e.g., a concrete mix of proportions

1:2:4 means that cement, fine and coarse

aggregate are in the ratio 1:2:4 or the mix contains

one part of cement, two parts of fine aggregate and

four parts of coarse aggregate. The proportions are

either by volume or by mass. The water-cement

ratio is usually expressed in mass

FACTORS TO BE CONSIDERED FOR MIX DESIGN

The grade designation giving the characteristic strength requirement of concrete.

The type of cement influences the rate of development of

compressive strength of concrete.

Maximum nominal size of aggregates to be used in

concrete may be as large as possible within the limits

prescribed by IS 456:2000.

The cement content is to be limited from shrinkage,

cracking and creep.

The workability of concrete for satisfactory placing and

compaction is related to the size and shape of section,

quantity and spacing of reinforcement and technique

used for transportation, placing and compaction.

I S CODE METHOD OF MIX DESIGN

19

C5

02

.6

PROCEDURE

1. Target strength for mean strength

The target mean compressive strength at 28 days

(ft) =fck+ K.S

K = a statistical value , usually taken as 1.65

S = standard deviation for each grade of

concrete ( table 8 of I.S. 456 -2000 )

20

C5

02

.6

21

Values of K

Accepted proportion of

low results K

1 in 5, 20% 0.84

1 in 10, 10% 1.28

1 in 15, 6.7% 1.50

1 in 20, 5% 1.65

1in 40, 2.5% 1.86

1 in 100, 1% 2.33

TABLE-8, IS CODE

Grade of concrete Assumed Standard ,

Deviations (N/mm )

M 10 ,M 15 3.5

M 20, M25 4.0

M 30, M 35, M 40,

M 45 & M 50

5.0

C5

02

.6

22

C5

02

.6

23

A) The free water cement

ratio corresponding to

the target strength is to

be determined from the

graph shown in fig.

2.Selection of water cement ratio :

Modified graph for Selection of water cement ratio :

Exposure Plain Concrete Reinforced Concrete

Min.

Cement

Max

w/c

Min

grade

Min.

Cement

Max

w/c

Min

grade

Mild

220

kg/m3 0.60 --

300

kg/m3

0.55 M 20

Moderate 240

kg/m3 0.60 M 15

300

kg/m3 0.50 M 25

Severe 250

kg/m3

0.50 M 20 320

kg/m3

0.45 M 30

V. Severe 260

kg/m3

0.45 M 20 340

kg/m3

0.45 M 35

Extreme 280

kg/m

0.40 M 25 360

kg/m

0.40 M 40

B) The water cement ratio, as selected above should be checked against the limiting water cement ratio for the durability requirements as given in table

Durability Criteria as per IS 456- 2000

Adjustments to minimum cement content for

aggregates other than 20 mm nominal max. size

aggregates as per IS 456: 2000.

10 mm + 40 kg/cum

20 mm

0

40 mm - 30 kg/cum

Placing

condition

Degree Slump

(mm)

Compaction

factor

Mass concrete,

lightly reinforced

sections in beams,

walls, columns and

floors

LOW 25 to 75 0.8 to 0.85

Heavily reinforced

sections in slabs,

beams, walls,

columns and

footings

MEDIUM 50 to 100 0.9 to 0.92

Slip formwork,

pumped concrete,

in- situ piling

HIGH 100 to 150 0.95 to 0.96

28

Approximate water content (Kg) per cubic metre of concrete (Table 32, SP:23-1982)

Slump

(mm)

Maximum Size of

Aggregate

(mm)

10 20 40

30-50 205 185 160

80-100 225 200 175

150-180 240 210 185

3.Estimation of entrapped air

Depends on nominal max size of aggregate as given in table

29

C5

02

.6

Max. size of aggregate (mm) Entrapped air as % of volume of

concrete

10 3.0

20 2.0

40 1.0

4. Selection of water content and fine to total aggregate ratio

The values are given in the tables, based on the following

conditions

(a) Crushed (Angular) Coarse aggregate conforming to IS: 383

(b) Sand conforming to grading zone II of table 4 of IS 383

(c) Workability corresponds to C.F. of 0.8 30

C5

02

.6

5.a. Approximate sand and water contents per cu.m of concrete

W/C = 0.6, Workability = 0.8 C.F. (For medium strength concrete up to M35)

Maximum size of

aggregate (mm)

Water content

including surface

water per m of

concrete (kg)

Sand as % of total

aggregate by

absolute volume

10

200 40

20

186 35

40 165 30

C5

02

.6

31

Step 5 - Estimation of Coarse Aggregate Proportion

For W/C ratio of 0.5 use following Table

Correction in Coarse Aggregate values The

table specified for W/C ratio of 0.5

1. For Every +0.05 change in W/C ratio: -0.01

2. For Every -0.05 change in W/C ratio: +0.01

3. For Pumpable Mix : -10 %

57

5.c. Adjustments of values in Water Content and sand %

for other conditions

Change in conditions stipulated

for tables

Adjustment required in

Water contents % sand in total

aggregate

For sand conforming to zone I

,zone III or zone Iv of I.S 383-

1979

0 +1.5%for zone I

-1.5% for zone III

-3.0 % for zone Iv

Increase or decrease in the value

of compacting factor by 0.1

3%

0

Each 0.05 increase or decrease in

water cement ratio

0

1.0 %

For rounded aggregates -15kg/m -7 %

C5

02

.6

34

For Other Conditions as per IS:10262,2009

Condition Correction

Sub-Angular Aggregates - 10 Kg

Gravel + Crushed Particles - 20 Kg

Rounded Gravel - 25 Kg

For every slump increase of

25 mm

+ 3 %

Use of Water Reducing

Admixture

- 5 to 10 %

Use of Superplasticzing

Admixtures

- 20 %

54

6.Determination of cement content

a) From free W/C ratio and

b) quantity water per unit volume of concrete for

workability (as derived in 5.c)

Cement by mass = (Water content) / (w.c.r.)

This cement content should not be less than

minimum content from the aspect of durability

(given in 2.b)

36

C5

02

.6

7.Calculation of aggregate content (fa and Ca)

37

C5

02

.6

where V = absolute volume of concrete

= gross volume (1m3) minus the volume of entrapped air

Sc = specific gravity of cement

W = Mass of water per cubic metre of concrete, kg

C = mass of cement per cubic metre of concrete, kg

p = ratio of fine aggregate to total aggregate by absolute

volume

fa, Ca = total masses of fine and coarse aggregates, per

cubic metre of concrete, respectively, kg, and

Sfa, Sca = specific gravities of saturated surface dry fine

and coarse aggregates, respectively

9. Determine the concrete mix proportions for the

first trial mix.

10. Prepare the concrete using the calculated

proportions and cast three cubes of 150 mm size

and test them wet after 28-days moist curing and

check for the strength.

11. Prepare trial mixes with suitable adjustments till

the final mix proportions are arrived at.

40

So the mix proportion works out to be

W : C : fa : ca

= 185 : 411 : 635 : 1150

= 0.45 : 1 : 1.55 : 2.80

This mix will be considered as Trial Mix No.2

41

Step VII:- Make slump trials to find out the actual weight of water to get required slump. Make corrections to the water content & %FA, if required. Step VIII:- Compute 2 more trial mixes with W/C ratios as 0.40 & 0.50, taking %FA as 34% and 38% respectively.

42

Trial Mix No. 1:-

Cement = 185 / 0.4 = 462.5 Kg.

Substituting the values in Eq(1), we get

1000 = 185 + 462.5/3.0 + (1/0.34) * fa /2.6)

fa = 584 Kg.

Substituting the values in Eq(2), we get

1000 = 185 + 462.5/3.0 + (1/0.66) * ca /2.65)

ca = 1156 Kg.

So the mix proportion works out to be

W : C : fa : ca

= 185 : 462.5 : 584 : 1156

= 0.4 : 1 : 1.26 : 2.50

43

Trial Mix No. 3:-

Cement = 185 / 0.5 = 370 Kg.

Substituting the values in Eq(1), we get

1000 = 185 + 370/3.0 + (1/0.38) * fa /2.6)

fa = 683 Kg.

Substituting the values in Eq(2), we get

1000 = 185 + 370/3.0 + (1/0.62) * ca /2.65)

ca = 1136 Kg.

So the mix proportion works out to be

W : C : fa : ca

= 185 : 370 : 683 : 1136

= 0.5 : 1 : 1.85 : 3.07

44

Step IX:- Cast atleast 3 cubes for each trial mix.

Step X:- Test the cubes for compressive strength at 28 days.

45

28 Days Compressive Strengths of Trial Mixes

W/C

Ratio C/W Ratio

Compressive

Strength

(Kg/Cm2)

0.40 2.50 457

0.45 2.22 420

0.50 2.00 360

46

Step XI:- Draw a graph between compressive strength Vs C/W Ratio.

47

48

Step XII:- From the graph, find the W/C ratio for the required target mean compressive strength. Step XIII:- Calculate the mix proportions corresponding to the W/C ratio, obtained from the graph.

49

Final Mix:-

From the graph, for a target strength of 390 Kg/Cm2, W/C ratio = 0.47

Cement = 185 / 0.47 = 394 Kg.

Substituting the values in Eq(1), we get

1000 = 185 + 394/3.0 + (1/0.38) * fa /2.6)

fa = 675 Kg.

Substituting the values in Eq(2), we get

1000 = 185 + 394/3.0 + (1/0.62) * ca /2.65)

ca = 1123 Kg.

So the mix proportion works out to be

W : C : fa : ca

= 185 : 394 : 675 : 1123

= 0.47 : 1 : 1.71 : 2.85

50

Step XIV:- Check the cement content & W/C ratio against the limiting values given in Table-5 of I.S: 456-2000 for given type of exposure & type of Concrete.

51

Table-5 Minimum Cement content Maximum Water-Cement ratio and Minimum Grade of Concrete for different exposures with normal weight of aggregate of 20mm nominal maximum size.

Sl. No.

Exposure

Plain Concrete Reinforced Concrete

Minimum Cement Content kg/m3

Maximum Free

Water Cement Ratio

Minimum Grade of Concrete

Minimum Cement Content kg/m3

Maximum Free

Water Cement Ratio

Minimum Grade of Concrete

i) Mild 220 0.60 - 300 0.55 M20

ii) Moderate 240 0.60 M15 300 0.50 M25

iii) Severe 250 0.50 M20 320 0.45 M30

iv) Very Severe

260 0.45 M20 340 0.45 M35

v) Extreme 280 0.40 M25 360 0.40 M40

52

From the table 5 of IS: 4562000, the minimum Cement content & W/C ratio, For moderate, for RCC are 300Kgs. & 0.5

The Cement content = 394Kgs. > 300Kgs. Hence Ok The W/C Ratio = 0.47 < 0.5 Hence Ok

53

TEST REPORT Concrete Mix RCC M30 with 20.0mm M.S.A.

Sl. No.

Particulars Result

1 Characteristic Compressive strength in N/Sq.mm

30

2 Maximum size of Aggregate in mm 20.0

3 Type of Exposure Moderate

4 Type of Site control Good

5 Target Average Compressive Strength in N/Sq.mm

38.2

6 Workability in terms of Slump in mm 25-75

7 Mode of Compaction Vibration

8 Mix Partiuclars: a. Water-Cement Ratio b. Materials per cubic metre of concrete in

Kg. i) Water ii) Cement (OPC 43 Grade) iii) Fine Aggregate iv) Coarse Aggregate c. Mix Portion by weight

0.47 185 394 675 1123

1:1.71:2.85

CONVERTING WEIGHT TO VOLUME

Unit weight of Cement =1440 Kg/mt3

Unit weight of F.A =1600 Kg/mt3

Unit weight of C.A =2200 Kg/mt3

1 bag of cement =1.25 cft

Proportions for Nominal Mix Concrete Grade of

Concrete Total qty of dry

aggregate (CA +

FA) per 50 kg

cement

Proportion of

FA to CA by

volume

Water per 50

kg cement

(max) lit

M 5 800

1: 2 (Zone II)

subject to upper

limit of 1: 1.5

(Zone I)

& lower limit of

1: 2.5 (Zone

III)

60

M 7.5 625 45

M 10 480 34

M 15 330 32

M 20 250 30 64

Example for Nominal Mixes

Grade of Concrete: M 20

Total Aggregate (CA + FA) per 50 kg cement: 250 kg, FA of Zone II (say)

Water content: 30 lit per 50 kg cement

w/c ratio= 30/50= 0.60

Considering FA: CA= 1: 2,

Sand= (250 X 1)/ 3= 83 kg

Coarse Aggregate= (250 X 2)/ 3= 167 kg

Cement FA CA Water

50 kg (35 Lit) 83 kg 167 kg 30 lit 65

Major Changes in : IS 10262

S,N

Old Edition 1982 Revised 2009 Edition

1 Title - " Recommanded guidelines for Concrete mix Desiqn11

Title - "Concrete mix Proportioning - Guidelines1

2 Applicability was not specified for any specific Concrete Grades

Specified for Ordinary (M 10 - M 20} and Standard (M25 - M 55) Concrete Grades only.

3 Based on IS 456 : 1982 Modification in iine with IS 456 : 2000

4

W / C ratio was based on Concrete grade and 28 days compressive strength of Concrete and the durability criteria

W/C ratio is based on Durability criteria and the Experience and Practical trials

5

Water Content could be modified taking into account the compaction factor value (Laboratory based test for Workability) and the shape of aggregates.

Water content can be modified Based on Slump vale (Field test of Workability) and Shape of Aggreagtes, and use of Admixtu res.

6 Entrapped Air cotent considered according to Nominal Maximum size of Aggregates

No Entrapped Air content taken into account

7 Not much Consideration for Trial Mixes

Trial Mixes concept is mentioned

e Concrete Mix Design with Fly ash is not mentioned

An illustrative example of Concrete Mix Prportioning using Fly ash has been added

Cement FA CA Water

50 kg 83 kg 167 kg 30 lit

(by weight) 1 1.66 3.32 0.6

1.43 kg/ lit 1.52 kg/ lit 1.60 kg/ lit 35 lit 54.6 lit 104.4 lit 30 lit

(by volume) 1 1.56 2.98

M 20 Grade Concrete (by Volume) is 1: 1.5 % : 3

66

Click here to load reader

Embed Size (px)

Recommended